#------------------------------------------------------------------------------
#$Date: 2016-02-20 02:53:41 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176768 $
#$URL: svn://www.crystallography.net/cod/cif/2/10/42/2104210.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2104210
loop_
_publ_author_name
'Michiue, Yuichi'
'Kimizuka, Noboru'
'Kanke, Yasushi'
_publ_section_title
;
 Structure of Ga₂O₃(ZnO)₆: a member of the homologous series
 Ga₂O₃(ZnO)ₘ
;
_journal_coeditor_code           KD5022
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              521
_journal_page_last               526
_journal_paper_doi               10.1107/S0108768108021125
_journal_volume                  64
_journal_year                    2008
_chemical_formula_sum            'Ga2 O9 Zn6'
_chemical_formula_weight         675.7
_chemical_name_systematic        ' ?'
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   3.2465(9)
_cell_length_b                   19.640(5)
_cell_length_c                   24.783(6)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    298
_cell_measurement_theta_max      15.7
_cell_measurement_theta_min      12.6
_cell_volume                     1580.2(7)
_computing_publication_material  '(Jana2000; Petricek and Dusek, 2000)'
_computing_structure_refinement  '(Jana2000; Petricek and Dusek, 2000)'
_diffrn_ambient_temperature      298
_diffrn_measured_fraction_theta_full 1.00
_diffrn_measurement_device_type  'Rigaku AFC-7R'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.1223
_diffrn_reflns_av_sigmaI/netI    0.1343
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       38
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       49
_diffrn_reflns_limit_l_min       -49
_diffrn_reflns_number            7287
_diffrn_reflns_theta_full        44.98
_diffrn_reflns_theta_max         44.98
_diffrn_reflns_theta_min         2.64
_diffrn_standards_decay_%        0.0
_diffrn_standards_interval_count 200
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    24.631
_exptl_absorpt_correction_T_max  0.61
_exptl_absorpt_correction_T_min  0.18
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   'Absorption correction given as psi-scan'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    5.679
_exptl_crystal_description       irregular
_exptl_crystal_F_000             2512
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.32
_refine_diff_density_min         -1.93
_refine_ls_extinction_coef       0.0078(3)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_ref   1.05
_refine_ls_number_parameters     113
_refine_ls_number_reflns         3699
_refine_ls_R_factor_all          0.1812
_refine_ls_R_factor_gt           0.0452
_refine_ls_shift/su_max          0.0331
_refine_ls_shift/su_mean         0.0033
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(σ²(I)+0.0001I²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0710
_refine_ls_wR_factor_ref         0.1005
_reflns_number_gt                1349
_reflns_number_total             3699
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            kd5022.cif
_cod_data_source_block           I
_cod_database_code               2104210
_cod_database_fobs_code          2104210
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 x,y,1/2-z
3 -x,y,z
4 -x,y,1/2-z
5 -x,-y,-z
6 -x,-y,1/2+z
7 x,-y,-z
8 x,-y,1/2+z
9 1/2+x,1/2+y,z
10 1/2+x,1/2+y,1/2-z
11 1/2-x,1/2+y,z
12 1/2-x,1/2+y,1/2-z
13 1/2-x,1/2-y,-z
14 1/2-x,1/2-y,1/2+z
15 1/2+x,1/2-y,-z
16 1/2+x,1/2-y,1/2+z
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_occupancy
Zn Zn1 0 0.00986(5) 0.06901(4) 0.0121(2) Uani d 1
Zn Zn2 0 0.13506(5) 0.61698(4) 0.0102(2) Uani d 1
Zn Zn3 0 0.12576(7) 0.75 0.0085(3) Uani d 1
Ga Ga4 0 0.38720(4) 0.00459(4) 0.01131(17) Uani d 1
Zn Zn5 0 0.36650(5) 0.62690(5) 0.0157(2) Uani d 1
Zn Zn6 0 0.51297(4) 0.68246(4) 0.00981(18) Uani d 1
Zn Zn7 0 0.36488(12) 0.75 0.0111(6) Uani d 0.528(4)
Zn Zn8 0 0.10969(19) 0.2564(4) 0.0311(19) Uani d 0.236(2)
Ga Ga9 0 0.24094(4) 0.05420(4) 0.01102(19) Uani d 1
Zn Zn10 0 0.25526(5) 0.18559(4) 0.0103(2) Uani d 1
O O1 0 0.4363(3) 0.5721(3) 0.0163(13) Uani d 1
O O2 0 0.4327(4) 0.25 0.0105(16) Uani d 1
O O3 0 0.0409(2) 0.8579(2) 0.0121(11) Uani d 1
O O4 0 0.0698(3) 0.5254(3) 0.030(2) Uani d 1
O O5 0.066(3) 0.4167(4) 0.8083(3) 0.025(2) Uiso d 0.5
O O6 0 0.3322(3) 0.0831(2) 0.0178(14) Uani d 1
O O7 0 0.1990(4) 0.25 0.020(2) Uani d 1
O O8 0 0.1901(3) 0.1255(2) 0.0128(12) Uani d 1
O O9 0 0.2979(2) 0.5265(3) 0.0198(15) Uani d 1
O O10 0 0.1888(2) 0.6871(2) 0.0094(12) Uani d 1
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga 0.231 1.608 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.1'
Zn 0.284 1.430 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.1'
O 0.011 0.006 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.1'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O1 Zn1 O1 14_454 14_554 113.70(19) no
O1 Zn1 O3 14_454 5_556 103.2(2) no
O1 Zn1 O4 14_454 6_554 118.09(18) no
O1 Zn1 O1 14_554 14_454 113.70(19) no
O1 Zn1 O3 14_554 5_556 103.2(2) no
O1 Zn1 O4 14_554 6_554 118.09(18) no
O3 Zn1 O4 5_556 6_554 95.8(3) no
O3 Zn2 O6 2_556 14_455 116.95(16) no
O3 Zn2 O6 2_556 14_555 116.95(16) no
O3 Zn2 O10 2_556 . 102.6(2) no
O6 Zn2 O6 14_455 14_555 113.8(2) no
O6 Zn2 O10 14_455 . 101.41(19) no
O6 Zn2 O6 14_555 14_455 113.8(2) no
O6 Zn2 O10 14_555 . 101.41(19) no
O2 Zn3 O2 13_456 13_556 109.5(2) no
O2 Zn3 O10 13_456 . 111.02(11) no
O2 Zn3 O10 13_456 2_556 111.02(11) no
O2 Zn3 O2 13_556 13_456 109.5(2) no
O2 Zn3 O10 13_556 . 111.02(11) no
O2 Zn3 O10 13_556 2_556 111.02(11) no
O10 Zn3 O10 . 2_556 103.2(2) no
O10 Zn3 O10 2_556 . 103.2(2) no
O1 Ga4 O4 2_555 14_454 92.3(3) no
O1 Ga4 O4 2_555 14_554 92.3(3) no
O1 Ga4 O6 2_555 . 177.9(2) no
O1 Ga4 O9 2_555 2_555 93.2(2) no
O4 Ga4 O4 14_454 14_554 117.3(3) no
O4 Ga4 O6 14_454 . 88.8(3) no
O4 Ga4 O9 14_454 2_555 121.06(18) no
O4 Ga4 O4 14_554 14_454 117.3(3) no
O4 Ga4 O6 14_554 . 88.8(3) no
O4 Ga4 O9 14_554 2_555 121.06(18) no
O6 Ga4 O9 . 2_555 84.6(2) no
O1 Zn5 O5 . 2_556 103.1(3) no
O1 Zn5 O5 . 4_556 103.1(3) no
O1 Zn5 O8 . 14_455 112.87(18) no
O1 Zn5 O8 . 14_555 112.87(18) no
O5 Zn5 O5 2_556 4_556 13.0(4) no
O5 Zn5 O8 2_556 14_455 113.7(3) no
O5 Zn5 O8 2_556 14_555 102.5(3) no
O5 Zn5 O5 4_556 2_556 13.0(4) no
O5 Zn5 O8 4_556 14_455 102.5(3) no
O5 Zn5 O8 4_556 14_555 113.7(3) no
O8 Zn5 O8 14_455 14_555 111.17(18) no
O8 Zn5 O8 14_555 14_455 111.17(18) no
O2 Zn6 O3 5_566 10_456 106.02(18) no
O2 Zn6 O3 5_566 10_556 106.02(18) no
O2 Zn6 O5 5_566 2_556 115.4(3) no
O2 Zn6 O5 5_566 4_556 115.4(3) no
O3 Zn6 O3 10_456 10_556 109.84(19) no
O3 Zn6 O5 10_456 2_556 115.1(3) no
O3 Zn6 O5 10_456 4_556 104.0(3) no
O3 Zn6 O3 10_556 10_456 109.84(19) no
O3 Zn6 O5 10_556 2_556 104.0(3) no
O3 Zn6 O5 10_556 4_556 115.1(3) no
O5 Zn6 O5 2_556 4_556 12.8(4) no
O5 Zn6 O5 4_556 2_556 12.8(4) no
O5 Zn7 O5 . 2_556 108.4(4) no
O5 Zn7 O5 . 3_555 13.8(5) no
O5 Zn7 O5 . 4_556 110.2(4) no
O5 Zn7 O7 . 13_456 116.4(3) no
O5 Zn7 O7 . 13_556 104.7(3) no
O5 Zn7 O5 2_556 . 108.4(4) no
O5 Zn7 O5 2_556 3_555 110.2(4) no
O5 Zn7 O5 2_556 4_556 13.8(5) no
O5 Zn7 O7 2_556 13_456 116.4(3) no
O5 Zn7 O7 2_556 13_556 104.7(3) no
O5 Zn7 O5 3_555 . 13.8(5) no
O5 Zn7 O5 3_555 2_556 110.2(4) no
O5 Zn7 O5 3_555 4_556 108.4(4) no
O5 Zn7 O7 3_555 13_456 104.7(3) no
O5 Zn7 O7 3_555 13_556 116.4(3) no
O5 Zn7 O5 4_556 . 110.2(4) no
O5 Zn7 O5 4_556 2_556 13.8(5) no
O5 Zn7 O5 4_556 3_555 108.4(4) no
O5 Zn7 O7 4_556 13_456 104.7(3) no
O5 Zn7 O7 4_556 13_556 116.4(3) no
O7 Zn7 O7 13_456 13_556 104.6(3) no
O7 Zn7 O7 13_556 13_456 104.6(3) no
O5 Zn8 O5 13_456 13_556 87.4(5) no
O5 Zn8 O5 13_456 14_454 74.0(3) no
O5 Zn8 O5 13_456 14_554 152.7(3) no
O5 Zn8 O5 13_456 15_456 7.6(3) no
O5 Zn8 O5 13_456 15_556 95.0(4) no
O5 Zn8 O5 13_456 16_454 80.7(3) no
O5 Zn8 O5 13_456 16_554 154.2(3) no
O5 Zn8 O7 13_456 . 98.6(3) no
O5 Zn8 O5 13_556 13_456 87.4(5) no
O5 Zn8 O5 13_556 14_454 150.0(4) no
O5 Zn8 O5 13_556 14_554 87.4(3) no
O5 Zn8 O5 13_556 15_456 79.8(5) no
O5 Zn8 O5 13_556 15_556 7.6(3) no
O5 Zn8 O5 13_556 16_454 150.4(4) no
O5 Zn8 O5 13_556 16_554 80.9(3) no
O5 Zn8 O7 13_556 . 99.8(4) no
O5 Zn8 O5 14_454 13_456 74.0(3) no
O5 Zn8 O5 14_454 13_556 150.0(4) no
O5 Zn8 O5 14_454 14_554 98.4(5) no
O5 Zn8 O5 14_454 15_456 80.9(3) no
O5 Zn8 O5 14_454 15_556 154.2(3) no
O5 Zn8 O5 14_454 16_454 7.5(3) no
O5 Zn8 O5 14_454 16_554 105.9(5) no
O5 Zn8 O7 14_454 . 106.0(3) no
O5 Zn8 O5 14_554 13_456 152.7(3) no
O5 Zn8 O5 14_554 13_556 87.4(3) no
O5 Zn8 O5 14_554 14_454 98.4(5) no
O5 Zn8 O5 14_554 15_456 150.4(4) no
O5 Zn8 O5 14_554 15_556 80.7(3) no
O5 Zn8 O5 14_554 16_454 90.9(5) no
O5 Zn8 O5 14_554 16_554 7.5(3) no
O5 Zn8 O7 14_554 . 108.7(4) no
O5 Zn8 O5 15_456 13_456 7.6(3) no
O5 Zn8 O5 15_456 13_556 79.8(5) no
O5 Zn8 O5 15_456 14_454 80.9(3) no
O5 Zn8 O5 15_456 14_554 150.4(4) no
O5 Zn8 O5 15_456 15_556 87.4(5) no
O5 Zn8 O5 15_456 16_454 87.4(3) no
O5 Zn8 O5 15_456 16_554 150.0(4) no
O5 Zn8 O7 15_456 . 99.8(4) no
O5 Zn8 O5 15_556 13_456 95.0(4) no
O5 Zn8 O5 15_556 13_556 7.6(3) no
O5 Zn8 O5 15_556 14_454 154.2(3) no
O5 Zn8 O5 15_556 14_554 80.7(3) no
O5 Zn8 O5 15_556 15_456 87.4(5) no
O5 Zn8 O5 15_556 16_454 152.7(3) no
O5 Zn8 O5 15_556 16_554 74.0(3) no
O5 Zn8 O7 15_556 . 98.6(3) no
O5 Zn8 O5 16_454 13_456 80.7(3) no
O5 Zn8 O5 16_454 13_556 150.4(4) no
O5 Zn8 O5 16_454 14_454 7.5(3) no
O5 Zn8 O5 16_454 14_554 90.9(5) no
O5 Zn8 O5 16_454 15_456 87.4(3) no
O5 Zn8 O5 16_454 15_556 152.7(3) no
O5 Zn8 O5 16_454 16_554 98.4(5) no
O5 Zn8 O7 16_454 . 108.7(4) no
O5 Zn8 O5 16_554 13_456 154.2(3) no
O5 Zn8 O5 16_554 13_556 80.9(3) no
O5 Zn8 O5 16_554 14_454 105.9(5) no
O5 Zn8 O5 16_554 14_554 7.5(3) no
O5 Zn8 O5 16_554 15_456 150.0(4) no
O5 Zn8 O5 16_554 15_556 74.0(3) no
O5 Zn8 O5 16_554 16_454 98.4(5) no
O5 Zn8 O7 16_554 . 106.0(3) no
O6 Ga9 O8 . . 97.7(2) no
O6 Ga9 O9 . 2_555 82.6(2) no
O6 Ga9 O9 . 14_454 120.11(14) no
O6 Ga9 O9 . 14_554 120.11(14) no
O8 Ga9 O9 . 2_555 179.8(2) no
O8 Ga9 O9 . 14_454 96.7(2) no
O8 Ga9 O9 . 14_554 96.7(2) no
O9 Ga9 O9 2_555 14_454 83.2(2) no
O9 Ga9 O9 2_555 14_554 83.2(2) no
O9 Ga9 O9 14_454 2_555 83.2(2) no
O9 Ga9 O9 14_454 14_554 115.4(2) no
O9 Ga9 O9 14_554 2_555 83.2(2) no
O9 Ga9 O9 14_554 14_454 115.4(2) no
O7 Zn10 O8 . . 104.6(3) no
O7 Zn10 O10 . 14_454 107.69(18) no
O7 Zn10 O10 . 14_554 107.69(18) no
O8 Zn10 O10 . 14_454 112.30(16) no
O8 Zn10 O10 . 14_554 112.30(16) no
O10 Zn10 O10 14_454 14_554 111.76(17) no
O10 Zn10 O10 14_554 14_454 111.76(17) no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Zn1 O1 14_454 1.939(3) yes
Zn1 O1 14_554 1.939(3) yes
Zn1 O3 5_556 2.068(6) yes
Zn1 O4 6_554 1.901(7) yes
Zn2 O3 2_556 1.951(5) yes
Zn2 O6 14_455 1.938(3) yes
Zn2 O6 14_555 1.938(3) yes
Zn2 O10 . 2.032(5) yes
Zn3 O2 13_456 1.988(4) yes
Zn3 O2 13_556 1.988(4) yes
Zn3 O10 . 1.991(5) yes
Zn3 O10 2_556 1.991(5) yes
Ga4 O1 2_555 2.131(6) yes
Ga4 O4 14_454 1.901(4) yes
Ga4 O4 14_554 1.901(4) yes
Ga4 O6 . 2.226(6) yes
Ga4 O9 2_555 1.915(5) yes
Zn5 O1 . 1.930(6) yes
Zn5 O5 2_556 1.898(8) yes
Zn5 O5 4_556 1.898(8) yes
Zn5 O8 14_455 1.968(3) yes
Zn5 O8 14_555 1.968(3) yes
Zn6 O2 5_566 1.985(4) yes
Zn6 O3 10_456 1.984(3) yes
Zn6 O3 10_556 1.984(3) yes
Zn6 O5 2_556 1.916(8) yes
Zn6 O5 4_556 1.916(8) yes
Zn7 O5 . 1.780(8) yes
Zn7 O5 2_556 1.780(8) yes
Zn7 O5 3_555 1.780(8) yes
Zn7 O5 4_556 1.780(8) yes
Zn7 O7 13_456 2.051(5) yes
Zn7 O7 13_556 2.051(5) yes
Zn8 O5 13_456 2.493(11) yes
Zn8 O5 13_556 2.196(12) yes
Zn8 O5 14_454 2.302(11) yes
Zn8 O5 14_554 1.977(11) yes
Zn8 O5 15_456 2.196(12) yes
Zn8 O5 15_556 2.493(11) yes
Zn8 O5 16_454 1.977(11) yes
Zn8 O5 16_554 2.302(11) yes
Zn8 O7 . 1.761(9) yes
Ga9 O6 . 1.930(6) yes
Ga9 O8 . 2.030(6) yes
Ga9 O9 2_555 2.290(6) yes
Ga9 O9 14_454 1.921(3) yes
Ga9 O9 14_554 1.921(3) yes
Zn10 O7 . 1.942(5) yes
Zn10 O8 . 1.964(6) yes
Zn10 O10 14_454 1.961(3) yes
Zn10 O10 14_554 1.961(3) yes
